Introduction to Fog/Rejuvenating Seals What are Fog and Rejuvenating Seals? Why use them? When to use them? Where to use them ?
What is a Fog Seal? A mixture of asphalt emulsion and water applied to the asphalt surface of a road, street or highway. The primary purpose is to seal the road surface and defer surface degradation.
Fog Seals - Description Light application of diluted slow-setting asphalt emulsion Common uses Seal aged surface Improve lane delineation Cost: 0.15 to 0.20 $/m 2 (0.12 to 0.17 $/yd 2 ) Typical treatment life: 1 to 2 years
A Fog Seal Job
Why Use Fog Seal? An inexpensive way of arresting raveling and adding binder back to aged surfaces Fog seals are also useful in chip seal applications to hold chips in place in fresh seal coats to help prevent vehicle damage arising from flying chips improve sealing or waterproofing improve the surface appearance
When to Use Fog Seal? Pavement surface condition – Dry mixes, high air voids, and surfaces showing minor and/or moderate raveling. When chip seals are in need to prevent aggregate loss. Pavement age – relatively newer pavement (not more than 2 years in service)
Where to Use Fog Seal? Pavement surface condition – Dry mixes, high air voids, and surfaces showing minor and/or moderate raveling. Pavement surface mix – can be used on dense-, gap-, and open-graded mixes; however, the seal must penetrate.
What is a Rejuvenating Seal? A combination of various chemicals or a mixture of asphalt emulsion and recycling agents applied to the asphalt pavement surface. The primary purpose is to soften the stiffness of the oxidized AC pavement surface and to extend the life of the pavement surface by adjusting properties of the AC mixture.
Why Use a Rejuvenating Seal? A way to soften the hardness of oxidized asphalt concrete surface, making it less brittle. The major benefit of the rejuvenating seals is to improve the flexibility of the asphalt binder and slow down the rate of aging and oxidization.
When to Use a Rejuvenating Seal? Old and fairly oxidized pavement surface or surface starting to oxidize or show raveling. In addition to oxidation a pavement surface may begin to show evidence of distress cracking; if this is the case a rejuvenating scrub seal should be used. Generally used on pavement over 2 years or more.
Where to Use Rejuvenating Seal? Can be used on dense-, gap- and open- graded pavement surface mixes Heavily aged, dense-graded HMA Open-graded HMA
Project Selection – Fog Seals Pavement surface condition – Dry mixes, high air voids, and surfaces showing minor and/or moderate raveling. Fog seal can also be used on chip seals to prevent aggregate loss. Pavement age – relatively newer pavement (not more than 2 years in service) Pavement surface mix – can be used on dense-, gap-, and open-graded mixes; however, the seal must penetrate.
Dense-graded HMA with closed surface Dense-graded HMA with closed surface Fog Seals - Unsuitable Surface
Fog Seals - Before and After Fog seal over existing chip seal
Project Selection – Rejuvenating Seals Pavement surface condition – old and fairly oxidized surface or surface starting to oxidize or show raveling. In addition to oxidation a pavement surface may begin to show evidence of distress cracking; if this is the case a rejuvenating scrub seal should be used. Pavement age – generally used on pavement over 2 years or more. Pavement surface mix – Can be used on dense-, gap- and open-graded mixes
Design Considerations The design objective is to determine the application rate and sometimes dilution rate. The actual application rates may vary during the construction.
Materials - What is an emulsion? Mixture of asphalt binder, water, and emulsifying agent 50 to 75% of mix is asphalt “Breaking” — separation of water and asphalt “Curing” — development of asphalt mechanical properties
Materials – General Terminology Original emulsion – A mixture of asphalt cement and water that contains a small amount of emulsifying agent. Original slow-setting grade emulsions contain up to 43 percent water and original rapid setting grade Diluted emulsion – An original emulsion that has been diluted by adding an amount of water equal to or more than the total volume of original emulsions contain up to 45 percent water. Residual asphalt content – The amount of asphalt remaining on the pavement surface after the emulsion has broken and cured (after all water has evaporated).
Materials – Fog Seals Usually asphalt emulsion and water. In some cases, the emulsions are made with a range of additives for special purposes. Emulsion types - may be Cationic (i.e., a positive surface charge on the asphalt particles), or Anionic (i.e., a negative surface charge on the asphalt particles). Primary types used: CSS-1h and SS-1h. In some circumstances, CQS-1h (and LMCQS-1h) will give a faster set.
Materials – Rejuvenating Seals They may be emulsions of rejuvenating additives and may include asphalt, polymers, and other additives Types of products commonly used in California Reclamite Emulsified Recycling Agent ( ERA ) Topein C Styraflex PASS
Materials – Rejuvenating Seals Reclamite - Emulsified recycling agent using heavy oils ERA - Emulsified recycling agent combined with a softer asphalt Topein C - Mixture of tall oil pitch, asphaltene resin, and petroleum asphalt emulsified with water Styraflex - Mixture of recycling agent, polymer and emulsified asphalt PASS - Mixture of recycling agent, polymer and emulsified asphalt
Specifications Fog Seals - NSSP Rejuvenating Seals - NSSP
Construction and Inspection From… Maintenance Technical Advisory Guide (MTAG) Module 7-2
Fog Seal Construction 1.Confirmation of Site Conditions 2.Surface preparation 3.Material preparation 4.Emulsion application 5.Sand blotter and sweeping (if necessary)
Confirmation of Site Conditions Consideration of site conditions is essential to proper curing Little or no chance of rain Temperature conditions Air: 5 °C (40 °F) Pavement: 15 °C (60 °F) Traffic control
Spray Bar and Nozzles Single Overlap Asphalt Distributor — Spray Bar Height h h Roadway Surface Double Overlap Roadway Surface Triple Overlap Roadway Surface h
15 o 45 o 90 o Travel Direction Lateral Coverage Asphalt Distributor — Spray Nozzles
Distributor Truck Applying a Seal
Post Treatment Procedures Sand blotter and sweeping (if necessary) Pavement should NOT be opened to traffic until adequate friction is restored
Rejuvenating Seal Construction Rejuvenator Application
Rejuvenating Seal Construction Application of Sand
Dos and Don’ts Do check water compatibility before dilution Do check dilution - has it been done, by whom, and when? Do ensure that there is no contamination of the base emulsion by water, oils, or other liquids. Do prevent contamination by other emulsions. Do protect emulsions from freezing or localized boiling due to the application of direct heat. Do heat emulsion gently and ensure heating coils are under the liquid level (max 122 F (50 C)). Do load from the bottom of tankers or sprayers to avoid foaming. Do check equipment and nozzles. Do check application rates. Do exercise proper traffic control. Do ensure the know-how is available on the job. Do add water to emulsion, not emulsion to water.
Dos and Don’ts Don’t store diluted emulsion longer than 24 hours. Don’t continuously stir or circulate emulsion. Don’t apply emulsion if air temperature is < 50°F (10 C) and pavement temperature < 60°F (15 C). Don’t apply emulsion if rain or cool temperatures are imminent. Don’t continue application if adequate breaking period is not available. Don’t open treated surface to traffic until coefficient of friction is at least 0.30 as determined by CT 342.
Troubleshooting - Approach Identify Problem Determine Cause Identify Solution
Troubleshooting Summary A=Anionic; C=Cationic
Common Problems and Related Solutions PROBLEMSOLUTION Spattering of the Emulsion Reduce the rate of dilution. Ensure the spray bar height is set correctly. Ensure the spray pressure is not set too high. Streaking of the Emulsion Ensure the emulsion is not too cold. Ensure the emulsion viscosity is not too high. Ensure the nozzles are at the same angle. Ensure the spray bar is not too high or too low. Ensure the spray bar pressure is not too high. Ensure all nozzles are not plugged. Bleeding or Flushing of the Emulsion Ensure the emulsion application rate is not too high. Check application and dilution rate and recalibrate sprayer, if necessary. Surface Coefficient of Friction is too Low per CT 342 Apply coating of clean dry sand. Sweep sand with rotary broom to absorb excess binder. Perform CT 342. Repeat process until coefficient of friction is at least 0.30.
Troubleshooting What is wrong here? Streaking
Troubleshooting What is wrong here? Non-Uniform Spray Distribution
Troubleshooting What is wrong here? Bleeding or Flushing
Problem: Sand not sticking Potential causes? Troubleshooting Possible Construction Problems
Problem: Excessive splattering of emulsion Potential causes? Troubleshooting Possible Construction Problems
Problem: Emulsion not breaking or breaking later than expected Potential causes? Troubleshooting Possible Construction Problems
Problem: Treatment washes off pavement Potential causes? Troubleshooting Possible Construction Problems
Problem: Treatment remains tacky, causing “pickup” by tires Potential causes? Troubleshooting Possible Construction Problems
Problem: Emulsion will not dilute Potential causes? Troubleshooting Possible Construction Problems
Problem: Emulsion breaking too fast Potential causes? Troubleshooting Possible Construction Problems
Summary Provided an overview of fog and rejuvenating seals Discussed design, materials, and specifications Discussed construction and inspection Discussed Dos and Don’ts Discussed problems and potential causes for troubleshooting